Polylactic acid, also known as poly(lactic acid) or polylactide (PLA), is a thermoplasticpolyester with backbone formula (C 3H 4O 2) n or [–C(CH 3)HC(=O)O–] n, formally obtained by condensation of lactic acidC(CH 3)(OH)HCOOH with loss of water (hence its name). It can also be prepared by ring-opening polymerization of lactide[–C(CH 3)HC(=O)O–] 2, the cyclic dimer of the basic repeating unit.
PLA has become a popular material due to it being economically produced from renewable resources. In 2010, PLA had the second highest consumption volume of any bioplastic of the world, although it is still not a commodity polymer. Its widespread application has been hindered by numerous physical and processing shortcomings. PLA is the most widely used plastic filament material in 3D printing. Its low melting point, high strength, low thermal expansion, good layer adhesion, and high heat resistance when annealed make it an ideal material for this purpose. Without annealing, however, PLA has the lowest heat resistance of the common 3D printing plastics.
Although the name "polylactic acid" is widely used, it does not comply with IUPAC standard nomenclature, which is "poly(lactic acid)". The name "polylactic acid" is potentially ambiguous or confusing, because PLA is not a polyacid (polyelectrolyte), but rather a polyester.
Several industrial routes afford usable (i.e. high molecular weight) PLA. Two main monomers are used: lactic acid, and the cyclic di-ester, lactide. The most common route to PLA is the ring-opening polymerization of lactide with various metal catalysts (typically tin octoate) in solution or as a suspension. The metal-catalyzed reaction tends to cause racemization of the PLA, reducing its stereoregularity compared to the starting material (usually corn starch).
The direct condensation of lactic acid monomers can also be used to produce PLA. This process needs to be carried out at less than 200 °C; above that temperature, the entropically favored lactide monomer is generated. This reaction generates one equivalent of water for every condensation (esterification) step. The condensation reaction is reversible and subject to equilibrium, so removal of water is required to generate high molecular weight species. Water removal by application of a vacuum or by azeotropic distillation is required to drive the reaction toward polycondensation. Molecular weights of 130 kDa can be obtained this way. Even higher molecular weights can be attained by carefully crystallizing the crude polymer from the melt. Carboxylic acid and alcohol end groups are thus concentrated in the amorphous region of the solid polymer, and so they can react. Molecular weights of 128–152 kDa are obtainable thus.
Another method devised is by contacting lactic acid with a zeolite. This condensation reaction is a one-step process, and runs about 100 °C lower in temperature.
Due to the chiral nature of lactic acid, several distinct forms of polylactide exist: poly-L-lactide (PLLA) is the product resulting from polymerization of L,L-lactide (also known as L-lactide).
Progress in biotechnology has resulted in the development of commercial production of the D enantiomer form.
Polymerization of a racemic mixture of L- and D-lactides usually leads to the synthesis of poly-DL-lactide (PDLLA), which is amorphous. Use of stereospecific catalysts can lead to heterotactic PLA which has been found to show crystallinity. The degree of crystallinity, and hence many important properties, is largely controlled by the ratio of D to L enantiomers used, and to a lesser extent on the type of catalyst used. Apart from lactic acid and lactide, lactic acid O-carboxyanhydride ("lac-OCA"), a five-membered cyclic compound has been used academically as well. This compound is more reactive than lactide, because its polymerization is driven by the loss of one equivalent of carbon dioxide per equivalent of lactic acid. Water is not a co-product.
PLA polymers range from amorphous glassy polymer to semi-crystalline and highly crystalline polymer with a glass transition 60–65 °C, a melting temperature 130-180 °C, and a Young's modulus 2.7–16 GPa. Heat-resistant PLA can withstand temperatures of 110 °C. The basic mechanical properties of PLA are between those of polystyrene and PET. The melting temperature of PLLA can be increased by 40–50 °C and its heat deflection temperature can be increased from approximately 60 °C to up to 190 °C by physically blending the polymer with PDLA (poly-D-lactide). PDLA and PLLA form a highly regular stereocomplex with increased crystallinity. The temperature stability is maximised when a 1:1 blend is used, but even at lower concentrations of 3–10% of PDLA, there is still a substantial improvement. In the latter case, PDLA acts as a nucleating agent, thereby increasing the crystallization rate.Biodegradation of PDLA is slower than for PLA due to the higher crystallinity of PDLA. The flexural modulus of PLA is higher than polystyrene and PLA has good heat sealability.
Several technologies such as annealing, adding nucleating agents, forming composites with fibers or nano-particles, chain extending and introducing crosslink structures have been used to enhance the mechanical properties of PLA polymers. Polylactic acid can be processed like most thermoplastics into fiber (for example, using conventional melt spinning processes) and film. PLA has similar mechanical properties to PETE polymer, but has a significantly lower maximum continuous use temperature.
Racemic PLA and pure PLLA have low glass transition temperatures, making them undesirable because of low strength and melting point. A stereocomplex of PDLA and PLLA has a higher glass transition temperature, lending it more mechanical strength.
The high surface energy of PLA results in good printability, making it widely used in 3D printing. The tensile strength for 3D printed PLA was previously determined.
PLA is soluble in a range of organic solvents.Ethyl acetate is widely used because of its ease of access and low risk. It is useful in 3D printers for cleaning the extruder heads and for removing PLA supports.
PLA-printed solids can be encased in plaster-like moulding materials, then burned out in a furnace, so that the resulting void can be filled with molten metal. This is known as "lost PLA casting", a type of investment casting.
PLA is used in a large variety of consumer products such as disposable tableware, cutlery, housings for kitchen appliances and electronics such as laptops and handheld devices, and microwavable trays. (However, PLA is not suitable for microwavable containers because of its low glass transition temperature.) It is used for compost bags, food packaging and loose-fill packaging material that is cast, injection molded, or spun. In the form of a film, it shrinks upon heating, allowing it to be used in shrink tunnels. In the form of fibers, it is used for monofilament fishing line and netting. In the form of nonwoven fabrics, it is used for upholstery, disposable garments, awnings, feminine hygiene products, and diapers.
PLA has applications in engineering plastics, where the stereocomplex is blended with a rubber-like polymer such as ABS. Such blends have good form stability and visual transparency, making them useful in low-end packaging applications.
PLA is used for automotive parts such as floor mats, panels, and covers. Its heat resistance and durability are inferior to the widely used polypropylene (PP), but its properties are improved by means such as capping of the end groups to reduce hydrolysis.
In the form of fibers, PLA is used for monofilament fishing line and netting for vegetation and weed prevention. It is used for sandbags, planting pots, binding tape and ropes .
PLA can degrade into innocuous lactic acid, making it suitable for use as medical implants in the form of anchors, screws, plates, pins, rods, and mesh. Depending on the type used, it breaks down inside the body within 6 months to 2 years. This gradual degradation is desirable for a support structure, because it gradually transfers the load to the body (e.g., to the bone) as that area heals. The strength characteristics of PLA and PLLA implants are well documented.
Thanks to its bio-compatibility and biodegradability, PLA found interest as a polymeric scaffold for drug delivery purposes.
The composite blend of poly(L-lactide-co-D,L-lactide) (PLDLLA) with tricalcium phosphate (TCP) is used as PLDLLA/TCP scaffolds for bone engineering.
Poly-L-lactic acid (PLLA) is the main ingredient in Sculptra, a facial volume enhancer used for treating lipoatrophy of the cheeks.
PLLA is used to stimulate collagen synthesis in fibroblasts via foreign body reaction in the presence of macrophages. Macrophages act as a stimulant in secretion of cytokines and mediators such as TGF-β, which stimulate the fibroblast to secrete collagen into the surrounding tissue. Therefore, PLLA has potential applications in the dermatological studies.
PLLA is under investigation as a scaffold that can generate a small amount of electric current via the piezoelectric effect that stimulates the growth of mechanically robust cartilage in multiple animal models.
PLA is degraded abiotically by three mechanisms:
Hydrolysis: The ester groups of the main chain are cleaved, thus reducing molecular weight.
Thermal decomposition: A complex phenomenon leading to the appearance of different compounds such as lighter molecules and linear and cyclic oligomers with different Mw, and lactide.
Photodegradation: UV radiation induces degradation. This is a factor mainly where PLA is exposed to sunlight in its applications in plasticulture, packaging containers and films.
The hydrolytic reaction is:
The degradation rate is very slow in ambient temperatures. A 2017 study found that at 25 °C in seawater, PLA showed no loss of mass over a year, but the study did not measure breakdown of the polymer chains or water absorption. As a result, it degrades poorly in landfills and household composts, but is effectively digested in hotter industrial composts, usually degrading best at temperatures of over 60 °C (140 °F).
Pure PLA foams are selectively hydrolysed in Dulbecco's modified Eagle's medium (DMEM) supplemented with fetal bovine serum (FBS) (a solution mimicking body fluid). After 30 days of submersion in DMEM+FBS, a PLLA scaffold lost about 20% of its weight.
PLA samples of various molecular weights were degraded into methyl lactate (a green solvent) by using a metal complex catalyst.
Four possible end-of-life scenarios are the most common:
Recycling: which can be either chemical or mechanical. Currently, the SPI resin identification code 7 ("others") is applicable for PLA. In Belgium, Galactic started the first pilot unit to chemically recycle PLA (Loopla). Unlike mechanical recycling, waste material can hold various contaminants. Polylactic acid can be chemically recycled to monomer by thermal depolymerization or hydrolysis. When purified, the monomer can be used for the manufacturing of virgin PLA with no loss of original properties  (cradle-to-cradle recycling).[dubious – discuss] End-of-life PLA can be chemically recycled to methyl lactate by transesterification.
Composting: PLA is biodegradable under industrial composting conditions, starting with chemical hydrolysis process, followed by microbial digestion, to ultimately degrade the PLA. Under industrial composting conditions (58 °C (136 °F)), PLA can partly (about half) decompose into water and carbon dioxide in 60 days, after which the remainder decomposes much more slowly, with the rate depending on the material's degree of crystallinity. Environments without the necessary conditions will see very slow decomposition akin to that of non-bioplastics, not fully decomposing for hundreds or thousands of years.
Incineration: PLA can be incinerated without producing chlorine-containing chemicals or heavy metals because it contains only carbon, oxygen, and hydrogen atoms. Since it does not contain chlorine it does not produce dioxins or hydrochloric acid during incineration. PLA can be combusted with no remaining residue. This and other results suggest that incineration is an environmentally friendly disposal of waste PLA.
Landfill: the least preferable option is landfilling because PLA degrades very slowly in ambient temperatures, often as slowly as other plastics.
^Vert M, Chen J, Hellwich KH, Hodge P, Nakano T, Scholz C, Slomkowski S, Vohlidal J. "Nomenclature and Terminology for Linear Lactic Acid-Based Polymers (IUPAC Recommendations 2019)". IUPAC Standards Online. doi:10.1515/iupac.92.0001.
^Martin O, Avérous L (2001). "Poly(lactic acid): plasticization and properties of biodegradable multiphase systems". Polymer. 42 (14): 6209–6219. doi:10.1016/S0032-3861(01)00086-6.
^ abSödergård A, Stolt M (2010). "3. Industrial Production of High Molecular Weight Poly(Lactic Acid)". In Auras R, Lim LT, Selke SE, Tsuji H (eds.). Poly(Lactic Acid): Synthesis, Structures, Properties, Processing, and Applications. pp. 27–41. doi:10.1002/9780470649848.ch3. ISBN978-0-470-64984-8.
^Jung YK, Kim TY, Park SJ, Lee SY (January 2010). "Metabolic engineering of Escherichia coli for the production of polylactic acid and its copolymers". Biotechnology and Bioengineering. 105 (1): 161–171. doi:10.1002/bit.22548. PMID19937727. S2CID205499487.
^Södergård A, Stolt M (February 2002). "Properties of lactic acid based polymers and their correlation with composition". Progress in Polymer Science. 27 (6): 1123–1163. doi:10.1016/S0079-6700(02)00012-6.
^Fiore GL, Jing F, Young Jr VG, Cramer CJ, Hillmyer MA (2010). "High Tg Aliphatic Polyesters by the Polymerization of Spirolactide Derivatives". Polymer Chemistry. 1 (6): 870–877. doi:10.1039/C0PY00029A.
^Urayama H, Kanamori T, Fukushima K, Kimura Y (1 September 2003). "Controlled crystal nucleation in the melt-crystallization of poly(l-lactide) and poly(l-lactide)/poly(d-lactide) stereocomplex". Polymer. 44 (19): 5635–5641. doi:10.1016/S0032-3861(03)00583-4. ISSN0032-3861.
^Tsuji H (1 January 1995). "Properties and morphologies of poly(l-lactide): 1. Annealing condition effects on properties and morphologies of poly(l-lactide)". Polymer. 36 (14): 2709–2716. doi:10.1016/0032-3861(95)93647-5. ISSN0032-3861.
^Urayama H, Ma C, Kimura Y (July 2003). "Mechanical and Thermal Properties of Poly(L-lactide) Incorporating Various Inorganic Fillers with Particle and Whisker Shapes". Macromolecular Materials and Engineering. 288 (7): 562–568. doi:10.1002/mame.200350004. ISSN1438-7492.
^Trimaille T, Pichot C, Elaissari A, Fessi H, Briançon S, Delair T (1 November 2003). "Poly(d,l-lactic acid) nanoparticle preparation and colloidal characterization". Colloid and Polymer Science. 281 (12): 1184–1190. doi:10.1007/s00396-003-0894-1. ISSN0303-402X. S2CID98078359.
^Hu X, Xu HS, Li ZM (4 May 2007). "Morphology and Properties of Poly(L-Lactide) (PLLA) Filled with Hollow Glass Beads". Macromolecular Materials and Engineering. 292 (5): 646–654. doi:10.1002/mame.200600504. ISSN1438-7492.
^Li BH, Yang MC (2006). "Improvement of thermal and mechanical properties of poly(L-lactic acid) with 4,4-methylene diphenyl diisocyanate". Polymers for Advanced Technologies. 17 (6): 439–443. doi:10.1002/pat.731. ISSN1042-7147.
^Di Y, Iannace S, Di Maio E, Nicolais L (4 November 2005). "Reactively Modified Poly(lactic acid): Properties and Foam Processing". Macromolecular Materials and Engineering. 290 (11): 1083–1090. doi:10.1002/mame.200500115. ISSN1438-7492.
^Nazre A, Lin S (1994). Harvey JP, Games RF (eds.). Theoretical Strength Comparison of Bioabsorbable (PLLA) Plates and Conventional Stainless Steel and Titanium Plates Used in Internal Fracture Fixation. p. 53. ISBN978-0-8031-1897-3.
^Lam CX, Olkowski R, Swieszkowski W, Tan KC, Gibson I, Hutmacher DW (2008). "Mechanical and in vitro evaluations of composite PLDLLA/TCP scaffolds for bone engineering". Virtual and Physical Prototyping. 3 (4): 193–197. doi:10.1080/17452750802551298. S2CID135582844.
^Ray S, Adelnia H, Ta HT (September 2021). "Collagen and the effect of poly-l-lactic acid based materials on its synthesis". Biomaterials Science. 9 (17): 5714–5731. doi:10.1039/d1bm00516b. PMID34296717.
^Pavia FC, La Carrubba V, Piccarolo S, Brucato V (August 2008). "Polymeric scaffolds prepared via thermally induced phase separation: tuning of structure and morphology". Journal of Biomedical Materials Research. Part A. 86 (2): 459–466. doi:10.1002/jbm.a.31621. PMID17975822.
^Gorrasi G, Pantani R (2017). "Hydrolysis and Biodegradation of Poly(lactic acid)". In Di Lorenzo ML, Androsch R (eds.). Synthesis, Structure and Properties of Poly(lactic acid). Vol. 279. Cham: Springer International Publishing. pp. 119–151. doi:10.1007/12_2016_12. ISBN978-3-319-64229-1.
^Iovino R, Zullo R, Rao MA, Cassar L, Gianfreda L (2008). "Biodegradation of poly(lactic acid)/starch/coir biocompositesunder controlled composting conditions". Polymer Degradation and Stabilit. 93: 147. doi:10.1016/j.polymdegradstab.2007.10.011.
^Pantani R, Sorrentino A (2013). "Influence of crystallinity on the biodegradation rate of injection-moulded poly(lactic acid) samples in controlled composting conditions". Polymer Degradation and Stability. 98 (5): 1089. doi:10.1016/j.polymdegradstab.2013.01.005.
^Chien YC, Liang C, Liu SH, Yang SH (July 2010). "Combustion kinetics and emission characteristics of polycyclic aromatic hydrocarbons from polylactic acid combustion". Journal of the Air & Waste Management Association. 60 (7): 849–855. doi:10.3155/1047-32126.96.36.1999. PMID20681432. S2CID34100178.